Patterns used in sand casting may be made of wood, metal, plastics or other materials. Patterns are made to exacting standards of construction, so that they can last for a reasonable length of time, according to the quality grade of the pattern being built, and so that they will repeatably provide a dimensionally acceptable casting.
The making of patterns, called patternmaking (sometimes styled pattern-making or pattern making), is a skilled trade that is related to the trades of tool and die making and moldmaking, but also often incorporates elements of fine woodworking. Patternmakers (sometimes styled pattern-makers or pattern makers) learn their skills through apprenticeships and trade schools over many years of experience. Although an engineer may help to design the pattern, it is usually a patternmaker who executes the design
Typically, materials used for pattern making are wood, metal or plastics. Wax and Plaster of Paris are also used, but only for specialized applications. Sugar pine is the most commonly used material for patterns, primarily because it is soft, light, and easy to work. Honduras Mahogany was used for more production parts because it is harder and would last longer than pine. Once properly cured it is about as stable as any wood available, not subject to warping or curling. Once the pattern is built the foundry does not want it changing shape. True Honduras Mahogany is harder to find now because of the decimation of the rain forests, so now there is a variety of woods marketed as Mahogany. Fiberglass and plastic patterns have gained popularity in recent years because they are water proof and very durable. Metal patterns are long lasting and do not succumb to moisture, but they are heavier, more expensive and difficult to repair once damaged.
Plaster of paris is usually used in making master dies and molds, as it gains hardness quickly, with a lot of flexibility when in the setting stage.
Sprues, gates, risers, cores, and chills or noEdit
The patternmaker or foundry engineer decides where the sprues, gating systems, and risers are placed with respect to the pattern. Where a hole is desired in a casting, a core may be used which defines a volume or location in a casting where metal will not flow into. Sometimes chills may be placed on a pattern surface prior to molding, which are then formed into the sand mould. Chills are heat sinks which enable localized rapid cooling. The rapid cooling may be desired to refine the grain structure or determine the freezing sequence of the molten metal which is poured into the mould. Because they are at a much cooler temperature, and often a different metal from what is being poured, they do not attach to the casting when the casting cools. The chills can then be reclaimed and reused.
The design of the feeding and gating system is usually referred to as methoding or methods design. It can be carried out manually, or interactively using general-purpose CAD software, or semi-automatically using special-purpose software (such as AutoCAST)
Types of PatternsEdit
Patterns are made of wood, metal, ceramic, or hard plastics and vary in complexity.
A single piece pattern, or loose pattern, is the simplest. It is a replica of the desired casting—usually in a slightly larger size to offset the contraction of the intended metal. Gated patterns connect a number of loose patterns together with a series of runners that will be detached after shake-out. Segmented or multi-piece patterns create a casting in several pieces to be joined in post-processing.
Match plate patterns are patterns with the top and bottom parts of the pattern, also known as the cope and drag portions, mounted on opposite sides of a board. This adaptation allows patterns to be quickly moulded out of the molding material. A similar technique called a cope and drag pattern is often used for large castings or large production runs: in this variation, the two sides of the pattern are mounted on separate pattern plates that can be hooked up to horizontal or vertical machines and moulded with the molding material. When the parting lines between the cope and drag are irregular, a follow board can be used to support irregularly shaped, loose patterns.
Sweep patterns are used for symmetric molds, which are contoured shapes rotated around a center axis or pole through the molding material. A sweep pattern is a form of skeleton pattern: any geometrical pattern that creates a mold by being moved through the molding material.
Skeleton pattern comes into play when the entire setup made of wood or metal is costlier. It is made usually as a part with some gaps left unfilled and those unfilled parts are filled or covered by loam sand or clays. Strickle board or Strike-off board is used to scrape the excess clay if applied to the gaps. Eg Turbine Casing, Soil and Water pipe bends, valve bodies and boxes.
To compensate for any dimensional changes which will happen during the (solid) cooling process, allowances are usually made in the pattern.
Almost all metals shrink volumetrically during solidification, this is known as liquid shrinkage. Another way of saying that is almost all metals undergo a volume increase upon melting, or liquidus temperature. Typical "volume shrinkage" is in the range between 3.5% to 10.0 % depending on the alloy. Some graphitic cast irons, when cast in heavier sections, under well controlled conditions, can exhibit a slight positive yield. Type Metal is also known, and used, for its ability to hold a true and sharp cast, and retain correct dimensions after cooling. Normally when making engineering cast parts the "method" is designed along with the pattern - being the riser size, number of risers, and location of risers. Additionally downsprue(s), runner bar(s), and ingate(s) are also designed in "the method". The "method" thus ensures the molten metal is delivered, the mould filled correctly, and the risers filled to "feed" the "shrinking volume" of liquid to the casting during solidification. This "method" is done by a "methods engineer", who may be a patternmaker (with additional training), a founding engineer, or metallurgist who is familiar with concept of volume increase / volume loss associated with melting and casting / solidification. Example: Assume steel at 7.85 density (solid) and 6% shrinkage, or better said, a 6% volume increase when molten. A mould has been made to cast a 100 kg block, based on the solid density of steel. The liquid density of steel is only 94% that of its solid density value - about 7.38 when liquid. Thus when the 100 kg block (solid calculation) is filled with liquid it contains a mass of only 94 kg. The 6kg, has to be supplied from a "riser" or "feeder" during solidification - thus the solid object now has a mass of 100 kg. The method is a system to deal with the volume loss during solidification. This (technically) is not an allowance.
After solidification has completed the dimensional size will then undergo linear contraction. This linear contraction proceeds right through cooling to room temperature. To compensate for this, the pattern is made larger than the required casting. This extra size that is given on the pattern for metal contraction is called "the contraction allowance". These values are typically between 0.6 % and 2.5 %. This is accounted for using a contraction rule, which is an oversized rule. Contraction rules are generally available for the common industrially cast alloys. Alternately, the Patternmaker will simply add a nominated percentage to all dimensions. An example of this allowance - if a bush were required to be 1500mm O/D, 1000mm I/D and 300mm high using a 2% contraction rule: The Patternmaker would make the pattern 1530mm O/D, (as it will contract in), 980 I/D (as the inside diameter will contract outwards) - important to note the Inside Diameter has 20mm "taken off it" rather than "added to it" - which is the correct contraction allowance. Finally, the height dimension would be 306mm.
The contraction amount can also be varied slightly by the sand system being used for the mould and any cores, for example clay-bonded sand, chemical bonded sands, or other bonding materials used within the sand. Exact values can vary between different foundries due to the sand systems being used. Each foundry, by gauging its own patterns and castings, can refine its own contraction allowances.
Shrinkage and Contraction can again be classified into liquid shrinkage and solid contraction. Liquid shrinkage is the reduction in volume during the process of solidification (liquid to solid), the liquid shrinkage is accounted for by risers. Solid contraction is the reduction in dimensions during the cooling of the (solid) cast metal. Contraction allowance takes into account only the solid contraction.
When the pattern is to be removed from the sand mold, there is a possibility that any leading edges may break off, or get damaged in the process. To avoid this, a taper is provided on the pattern, so as to facilitate easy removal of the pattern from the mold, and hence reduce damage to edges. The taper angle provided is called the Draft angle. The value of the draft angle depends upon the complexity of the pattern, the type of molding (hand molding or machine molding), height of the surface, etc. Draft provided on the casting is usually 1 to 3 degrees on external surfaces (5 to 8 internal surfaces).
Finishing or Machining allowanceEdit
The surface finish obtained in sand castings is generally poor (dimensionally inaccurate), and hence in many cases, the cast product is subjected to machining processes like turning or grinding in order to improve the surface finish. During machining processes, some metal is removed from the piece. To compensate for this, a machining allowance (additional material) should be given in the casting. the amount of finish allowance depends on the material of the casting, size of casting, volume of production, method of molding, etc.
Usually during removal of the pattern from the mold cavity, the pattern is rapped all around the faces, in order to facilitate easy removal. In this process, the final cavity is enlarged. To compensate for this, the pattern dimensions need to be reduced. There are no standard values for this allowance, as it is heavily dependent on the personnel. This allowance is a negative allowance, and a common way of going around this allowance is to increase the draft allowance. Shaking of the pattern causes an enlargement of the mould cavity and results in a bigger casting.
During cooling of the mould, stresses developed in the solid metal may induce distortions in the cast. This is more evident when the mould is thinner in width as compared to its length. This can be eliminated by initially distorting the pattern in the opposite direction.
Patterns continue to be needed for sand casting of metals. For the production of gray iron, ductile iron and steel castings, sand casting remains the most widely used process. For aluminum castings, sand casting represents about 12% of the total tonnage by weight (surpassed only by die casting at 57%, and semi-permanent and permanent mold at 19%; based on 2006 shipments). The exact process and pattern equipment is always determined by the order quantities and the casting design. Sand casting can produce as little as one part, or as many as a million copies.
Although additive manufacturing modalities such as SLS or SLM have potential to replace casting for some production situations, casting is still far from being completely displaced. Wherever it provides suitable material properties at competitive unit cost, it will remain in demand.
|Wikimedia Commons has media related to Casting patterns.|
- Bawa, H S (2004). Manufacturing Processes – I. Tata McGraw-Hill. pp. 1–12. ISBN 978-0-07-058372-6.
- Ammen, C. W. (1999). Metalcasting. McGraw-Hill Professional. pp. 159–176. ISBN 978-0-07-134246-9.
- Shelly, Joseph Atkinson. Patternmaking: A treatise on the construction and application of patterns, including the use of woodworking tools, the art of joinery, wood turning, and various methods of building patterns and core-boxes of different types.The common types of patterns are: 1) Single piece pattern 2) Split piece pattern 3) Loose piece pattern 4) Gated pattern 5) Match pattern 6) Sweep pattern 7) Cope and drag pattern 8) Skeleton pattern 9) Shell pattern 10) Follow board pattern 11) segmental pattern New York: Industrial Press, 1920; pp. 2-5 et seq
- Radhakrishna, K (2011). Manufacturing Process - 1. Bangalore: Sapna Book House. p. 20. ISBN 978-81-280-0207-6.
- Praveen, Kestoor (2011). Manufacturing process - 1. Bangalore: Star – tech education. p. 16.
- Rao, P.N. (2003). Manufacturing Technology. New Delhi: Tata McGraw-Hill. p. 68. ISBN 0-07-463180-2.